FACULTY OF SCIENCE AND TECHNOLOGY
Mathematics and Physics/Physics
Spring semester, 2020 Open
Eli Drange Vee Supervisor:
Title of master’s thesis:
X-ray Studies on partially decomposed γ- Mg(BH4
Credits (ECTS): 60 Keywords:
X-ray physics γ- Mg(BH4
X-ray absorption spectroscopy X-ray diffraction
Number of pages: 58
This is the final report of the research work of the master’s thesis carried out through 2019 fall and 2020 spring semesters to complete the master’s Program in Physics from the Department of Mathematics and Physics, University of Stavanger. The research subject is within Materials’ science and is focused on the study of a hydrogen storage material with common X-ray techniques such as X- ray absorption spectroscopy (XAS) and powder X-ray diffraction (PXD).
Stavanger, Norway, 15th July 2020 Rashmi Dahal
The master’s thesis has been submitted successfully on 15.07.2020. I would like to express my sincere gratitude to my supervisor, associate professor Dr. Olena Zavorotynska for her continuous encouragement and guidance with needed articles, books, useful hints and tips during the whole period of the thesis. I have been lucky to have a supervisor who always cared about my work and responded to my queries so promptly. I am deeply indebted to her as she is the one who opened the door of my experimental physics world through this thesis.
I would like to recognize the assistance that I received from our research lab engineer Ms. Anna Cecilie Åsland for the support to operate all the laboratory instruments and the corresponding software. I had a great time working with her.
A heartful thanks go to my husband, Mr. Milan Sanjel who always supported and nurtured me and always had a profound belief in my abilities.
A special thanks goes also to my family for making my idea of studying abroad possible. Especially my brother, Mr. Upendra Dahal who inspired me and supported all the times for this master’s studies.
I greatly appreciate Dr. Stefano Deledda from the Institute for Energy Technology (Norway) for providing the gamma phase magnesium borohydride sample for the whole work.
Thanks go to all the professors from the Department of Mathematics and Physics, the physical and technical contribution of the University of Stavanger for providing the educational platform for my whole master’s studies. The financial support for traveling to the synchrotrons is greatly appreciated.
XAS data for this experiment was collected on RGBL beamline at the BESSY II electron storage ring operated by the Helmholtz-Zentrum Berlin. I would particularly like to acknowledge the help and support of research scientists Anna Makarova and Dmitry Smirnov during the experiment and the financial support provided by the Synchrotron.
I must thank Synchrotron Elettra, Trieste, Italy for the funding that was provided even though the experimental part could not be carried out due to the technical problems in the Synchrotron.
Rashmi Dahal, 15th July, 2020
Hydrogen is the energy that fuels the sun and the stars. Having the potential to be zero-carbon during production, when produced by renewable resources, it is an attractive carrier of the pollution-free renewable energy. In this context, magnesium borohydride (Mg(BH4)2) is recognized as an attractive potential hydrogen storage material due to its high hydrogen content and low H2 release temperature.
Hydrogenation of completely decomposed Mg(BH4)2 requires high-temperature, high H2 pressure, and very long reaction time. Studies show that the partially decomposed Mg(BH4)2 can be hydrogenated in comparatively lower temperatures, pressure, and short reaction time but up to date, the reversible reaction shows only 2.5 wt% of H2 production which is not sufficient for its practical use. To achieve higher wt% of H2 it is important to understand the kinetics of the dehydrogenation and re- hydrogenation of Mg(BH4)2 reactions and the nature of the reaction intermediates. The latter has been debated for more than 10 years.
In this work, we decomposed γ-Mg(BH4)2 at different temperatures between 240-400°C. The composites have been analyzed by using combined thermogravimetric analysis and differential scanning calorimetry (TGA-DSC), X-ray absorption spectroscopy (XAS), and powder X-ray diffraction (PXD) techniques. 11.3 wt% of H2 desorption at 400°C was observed by gravimetric measurements.
PXD showed no crystalline decomposition products when heated between 260-280°C. X-ray absorption near edge structure (XANES) at B K-edge studies was carried out at RGBL, BESSY II, Berlin.
The qualitative analysis of the obtained data showed the tetrahedral B co-ordination in the samples decomposed between 240-300 °C and a combination of tetrahedral B with the B-H amorphous species in the reaction products formed in the 300-400°C temperature range. The XANES data also revealed the presence of amorphous boron above 340°C. In this way, this study has provided more insights into the decomposition reaction of Mg(BH4)2. The overall conclusion collected from combined TGA/DSC, PXD, and XAS data analysis have been presented as follows;
163℃→ ht1-Mg(BH4)2 195℃
→ ht2 -Mg(BH4)2 240 ℃
→ β- Mg(BH4)2 (XAS) + am.ph B-H (PXD) + 0.4 H2 (TGA) 260℃→ am. Ph B-H (XAS,PXD) + 0.6 H2 (TGA) 280℃→ am.ph B(?) (XAS, PXD) + am. ph B-H(?) (XAS, PXD) + H2 (TGA) 300℃→ am.ph B (XAS) + am. ph B-H(?) (XAS, PXD) + α- MgH2 + 1.6 H2 (TGA)320℃→ Mg + MgO (PXD) + am.ph B (?)+ am. ph B-H(?) (XAS, PXD) +2.5 H2(TGA) 340℃→ Mg + MgO (PXD) + am.ph B (XAS) + am. ph B-H(?) (XAS, PXD) +2.9 H2 (TGA) 400℃→ Mg (PXD) + am.ph B (XAS,PXD) + am. ph B-H(?) (XAS, PXD) +3.1 H2 (TGA)
1.1. Purpose of the thesis 1.2. Objectives
1.3. Background 2. Theory
2.1. X-rays wave-particle duality 2.2. X-ray production
2.2.1. X-ray production in Cathode tube 2.2.2. X-ray production in Synchrotron
2.3. X-ray spectroscopy and Interaction of X-rays with matter 2.4. X-ray absorption spectroscopy (XAS)
2.4.1 Introduction 2.4.2 Absorption process
2.4.3 Quantum mechanical treatment
22.214.171.124 Free electron approximation
126.96.36.199 Beyond free-electron approximation 2.4.4 Absorption edges
2.4.5 X-ray absorption spectroscopy (XANES) 2.4.6 Interpretation of XANES
2.4.7 Measurement modes of XANES 2.5. X-ray diffraction (XRD)
3.1. Experimental details 3.2. TGA and DSC instrument 3.3. Glove box
3.4. Synchrotron Beamline and XANES instrument 3.4.1 Sample Holders
3.4.2 XANES instrument 3.5. X-ray Diffraction instrument 4. Data Processing and analysis
4.1. TGA-DSC data analysis 4.2. XRD data analysis 4.3. XANES data analysis 5. Conclusion and future perspectives 6. References
1.1.Purpose of the thesis
The major purpose of this work is to study the partial decomposition reaction of magnesium borohydride as a hydrogen storage material. Mainly to study and analyze the intermediate reaction products when the magnesium borohydride is heated from the temperature between 240-400°C. The experimental analysis methodologies include decomposition and data reduction from combined thermogravimetric analysis and differential scanning calorimetry (TGA-DSC) technique, X-ray absorption spectroscopy (XAS), and the X-ray diffraction (XRD).
Magnesium borohydride (Mg(BH4)2) is One of the interesting materials for hydrogen storage due to its high hydrogen content and the lowest temperature of hydrogen release. In this work, magnesium borohydride will be partially decomposed between 240-400 °C temperature range, and the decomposed reaction product will be studied and analyzed with the thermogravimetric analysis (TGA) and differential scanning calorimetry (DSC) techniques. Furthermore, it will also be studied through the X-ray absorption spectroscopy (XAS) and the powder X-ray diffraction (PXD) techniques in order to identify the intermediate compounds through its weight loss, absorption edge, and the diffraction peaks of the compound formed after the partial decomposition of magnesium borohydride. Through this whole thesis, the following objectives are expected to be fulfilled;
• To carry out experiments and data analysis using TGA-DSC techniques.
• To handle and work well with air-sensitive samples using a glove box.
• To carry out the experiment on X-ray spectroscopy (XAS) and its data analysis.
• To work experimentally on powder X-ray diffraction (PXD) and its data analysis.
• To analyze the data obtained from TGA-DSC, XAS, and PXD using their corresponding software.
• To learn to work in a lab with great responsibility.
• To learn to discuss the results and their consequences to enhance future measurements.
• To learn scientific writing and literature search.
1.3. Background: Magnesium borohydride as a hydrogen storage material 1.3.1. Storing hydrogen in borohydrides
Although the technology of renewable energy utilization such as solar and wind energy, has been researched a lot, instability of the sources for these energies leads to the simultaneous operation of backup power systems. Also, at present, several major industries are currently looking to reduce their dependence on fossil fuels. In the pursuit to find solutions in both of these cases, the hydrogen storage concept surely plays an important role as a renewable source of energy.
Hydrogen is one of the most abundant, but highly flammable elements. It is lightweight, small in size, and a pollution-free energy carrier that is characterized by flexible and efficient energy conversion.
However, the low density of hydrogen gas, low temperature of its liquefication as well as high explosive risk are the major problems of the deVelopments of effective and safe hydrogen storage systems. At present, these problems related to safe and efficient have exceeded the deVelopment of hydrogen power engineering and technology. Besides these, all difficulties and the problems with hydrogen storage scientists have been able to discover the methods for hydrogen storage in some physical and
chemical methods including adsorption and absorption. The diagram below shows the recent methods of hydrogen storage in different ways.
Figure 1.1: The applied categorization of hydrogen storage technology 
Hydrogen can be stored by physical methods that contain H2 molecule which does not react with the storage medium. In the physical method, the hydrogen is stored as a compressed gas in gas cylinders, stationary storage systems including underground reservoirs, hydrogen storage in pipelines, and glass microspheres whereas in liquid form, hydrogen is stored as stationary and mobile cryogenic reservoirs.
In the chemical methods, hydrogen storage is done using the physical-chemical process of its interaction with some materials. The methods are characterized by an essential interaction of molecular or atomic hydrogen with the storage environment. These chemical methods include the storage of hydrogen as metal and chemical hydrides. Adsorption and absorption are the material- based hydrogen storage methods. In adsorption, the hydrogen is attached to the surface of material either as hydrogen molecules or as hydrogen atoms. In absorption, the hydrogen is stored within the solids. In absorption, hydrogen is dissociated into H-atoms and then the hydrogen atoms are fused into the solid lattice framework. Absorption in complex hydrides may make it possible to store a larger amount of hydrogen in smaller volumes at low pressure and temperatures close to room temperatures. Finally, hydrogen can be strongly bound within molecular structures as chemical compounds containing hydrogen atoms[1-3]
The table below (Table 1.1) shows the comparison between the different hydrogen storage methods.
Among all the methods, the metal hydrides and metal borohydride have high volumetric and gravimetric densities. It is important to recall that the efficiency of hydrogen storage for material depends on several components but usually mainly measured by two parameters, the gravimetric density, and the volumetric density. Gravimetric density referred to the weight % of hydrogen stored the total weight of the system (hydrogen + container) whereas the volumetric density referred to the stored hydrogen mass per unit volume of the system [1, 3].
Practically, the considerable energy losses, expensive storage tanks, and the safety risks are the main challenges associated with the Liquid and pressurized hydrogen tanks . Therefore, almost ten years ago the alkaline and alkaline earth metals borohydrides got the attention as hydrogen storage materials due to their high hydrogen content .
Method Gravimetric Energy Density (Wt %)
Volumetric Energy Density
Compressed 5.7 4.9 293 700 Current industry
Liquid 7.5 6.4 20 0 Boil-off constitutes
major disadvantage Cold/
5.4 4.0 40-80 300 Boil-off constitutes
MOF 4.5 7.2 78 20-100 Attractive densities
only at very low temperatures Carbon
2.0 5.0 298 100 Volumetric density
based on powder density of 2.1 g/mL and 2.0 wt% storage capacity.
Metal hydrides 7.6 13.2 260-425 20 Requires thermal
management system Metal
14.9-18.5 9.8-17.6 130 105 Low temperature, high
pressure thermal management required
Kubas-type 10.5 23.6 293 120
LOHC 8.5 7 293 0 Highly
endo/exothermal requires processing plant and catalyst. Not suitable for mobility.
Chemical 15.5 11.5 298 10 Requires SOFC fuel cells
Table 1.1: The comparison between the different hydrogen methods 
In the present work, we mainly focus on magnesium borohydride (Mg(BH4)2) and its characteristics, which made it more interesting hydrogen storage material than other metal borohydrides. Hydrogen storage property of magnesium borohydride could make it a promising and eVerlasting resource of clean and renewable energy as a replacement for fossil fuel. It can be used in fuel cells and the form of many other energies and can widely use for industrial purposes as well as according to [6, 7], this compound can further lead to magnesium rechargeable batteries.
The table below shows how Mg(BH4)2 stands out among other metal borohydrides from its gravimetric and volumetric densities point of view.
9 Hydrogenated form Dehydrogenated
-△H, kJ/mol H2
Decomposition temp. ºC
LiBH4 LiH + B 13. 93 75 402 470
2 LiBH4 +MgH2 3 LiH+ MgB2 11.4 46 225 315
2 LiBH4 + Al 2 LiH + AlB2 8.6 188
7 LiBH4 + 1.75 Mg2Sn + 0.25 Sn Li7Sn2 + 3.2 MgB2 6.3 46 184
NaBH4 NaH + B 7.9 85.5 90 609 595
2 NaBH4 + MgH2 3 NaH + MgB2 7.8 62 351
Be(BH4)2 Be + 2B 20.8 126 27 123
Mg(BH4)2 Mg + 2B 14.9 113 40 323
Ca(BH4)2 2/3 CaH2 + 1/3 CaB6 9.7 108 75.5 360
Ca(BH4)2 + MgH2 CaH2 + MgB2 8.3 159
Zn(BH4)2 Zn +2B* 8.5 85
Al(BH4)3 Al + 3B* 16.9 121 6 150
Sc(BH4)3 ScB2 + B (?) 13.5 260
Ti(BH4)3 TiB2 + B* 13.1 25
Mn(BH4)2 Mn + 2B 9.5
Zr(BH4)4 ZrB2 + 2B (?) 10.7 108 250
Table 1.2: Comparison between the gravimetric and volumetric densities of metal hydrides .
For any compound to work as hydrogen storage material, besides the gravimetric and volumetric densities they are supposed to have a low temperature of dehydrogenation and moderate or easy reVersibility of dehydrogenation, low working pressure, fast kinetics of desorption and absorption and high purity of released and reabsorbed hydrogen gas [4, 8]. Following these facts, among other borohydrides, Mg(BH4)2 turns out to be better. From the table above, it can be seen that, among other metal borohydrides, beryllium borohydride and magnesium borohydrides have much better gravimetric and volumetric densities. But beryllium oxide is too toxic for practical applications leaving magnesium borohydride as important hydrogen storage material.
Magnesium borohydride was first synthesized in the 1950s, but the interest in hydrogen energy made it a possible candidate for hydrogen storage . Magnesium borohydride (Mg(BH4)2) has the most complex crystal structures and the largest number of phase polymorphs among other borohydrides.
Among all known hydrides, Some of the polymorphs of Mg(BH4)2 contain a noteworthy porosity and also ultra-density with the second-highest volumetric hydrogen . Magnesium borohydride exists in various crystalline forms, as recently discovered and characterized by X-ray and neutron scattering techniques. Among the observed polymorphs of Mg(BH4)2, namely α, β, γ and δ-phase, the low- temperature (LT) α-phase and the high-temperature (HT) β-phase are the most commonly investigated for hydrogen storage applications . Many studies have been made to describe the synthesis and the crystal structure of magnesium borohydride which are explained in [7, 9-14].
In the present work, we are going to discuss the γ- Mg(BH4)2 phase as this is one that possesses a high porosity of almost 30% of open space in the structure . According to the author of  γ- Mg(BH4)2
has a cubic crystal structure with space group Ia-3d and Id-3a, and it is an interesting first example of porous high surface area complex hydride, which can absorb small molecules. The reported values of specific surface area (SSA) for γ- Mg(BH4)2 vary greatly between 60 to 1160 m2g-1. This property of γ- Mg(BH4)2 eventually can lead to new possible applications where surface effects are important.
γ- Mg(BH4)2 is the interest of the study from the hydrogen storage point of view because it contains 14.9 weight % of hydrogen and has suitable thermodynamics  and is more abundant than Li . It contains hydrogen-rich molecular anions (BH4)- - and the (Mg)++ cations. The gravimetric and volumetric hydrogen densities in this compound are even suitable for the demanding onboard hydrogen storage applications.Mg(BH4)2 can be decomposed between 215-410°C with mainly the release of hydrogen and also reaction is reversible in this temperature range . It has the lowest decomposition temperature among LiBH4, Be(BH4)2 and Mg(BH4)2 and all the group I and II borohydrides, and has the modest conditions for partial re-hydrogenation among all borohydrides as demonstrated experimentally on . This is the clear reason why composites based on Mg(BH4)2 are extensively studied fundamentally and are applicable as hydrogen storage materials . Recent studies on Mg(BH4)2 have revealed a more complex multistep decomposition pathway than previously thought, which suggests the formation of B-H amorphous intermediates similar in structure to MgB12H12. Besides these, studies have also shown an inverse correlation between the electronegativity of the cation and borohydride stability .
The partial and the complete reversible decomposition of Mg(BH4)2 has been studied using various experimental techniques such as combined thermogravimetric analysis and differential scanning calorimetry (TGA-DSC), X-ray diffractions (XRD), Fourier transform infrared radiation (FTIR), Raman, X- ray absorption spectroscopy (XAS), etc. The studies show that the re-hydrogenation of completely decomposed Mg(BH4)2 requires high temperature, high hydrogen pressure, and long reaction time.
However, the partially decomposed Mg(BH4)2 compounds can be re-hydrogenated in much milder conditions.
1.3.2 Hydrogen desorption and absorption in Mg(BH4)2
Desorption is the phenomenon where a substance is released from or through a surface of a solid and escape into the surrounding. The process is opposite to sorption which includes adsorption and absorption. These two properties are very important for a compound to work as a hydrogen storage material . Magnesium borohydride is predicted to have favorable thermodynamics which would allow hydrogen desorption at a temperature below 100°C. But, experiments show that the decomposition of Mg(BH4)2 requires at least 200°C. However, the decomposition process of Mg(BH4)2
suggests multiple reaction pathways with the unknown intermediates reaction products. Re- hydrogenation of completely decomposed Mg(BH4)2 is difficult to use for practical purposes as stated earlier but the re-hydrogenation of the intermediate reaction products obtained from the decomposition of γ- Mg(BH4)2 300°C, it is possible to produce with up to 2.8 wt% of H2. During the decomposition of highly crystalline γ- Mg(BH4)2 between 145-215°C, there is a phase transition from γ→ ε → β and then the decomposition starts. From 215-330°C, the first hydrogen desorption can be observed along with the appearance of amorphous B-H species. In the next stage, the formation of crystalline MgH2 takes place between 340-355°C which is then followed by the formation of amorphous boron (B) at a temperature between 355-372°C and the decomposition of MgB2 from 372- 420°C. According to the author of , there forms an undesirable by-product of diborane detected at temperature 280°C with various amorphous B-H species desorbed H2 and interacted with each other in multiple steps of complex magnesium borohydride decomposition procedure. The partial decomposition reaction of Mg(BH4)2 in a vacuum, hydrogen backpressure, and Argon (Ar) was studied in  which suggests that before the formation of MgB2 above 280°C, Mg(BH4)2 decomposed to MgxByHz amorphous reaction products with up to 6.8 wt% loss and overall reaction pathway of the experiment has been summarised by equation (1.1) given below,
→ MgB2H4.3 + 1.8 H2 (1.1)
Here are some important steps during the decomposition of γ- Mg(BH4)2 with some maintained reaction environment that is mentioned in [5, 7]
→ ε- Mg(BH4) (1.2)
ε- Mg(BH4) 165−215℃→ β - Mg(BH4) (1.3) γ- Mg(BH4)2
→ amorphous species (MgB12H12 + other polyborane species) + H2
→ MgH2 365−410℃
→ Mg + H2 (1.4)
→ amorphous species/melt 310−370℃→ MgH2 340−570℃→ Mg 490−600℃→ MgB2 (1.5)
Many experimental reports have shown that in every decomposition step the amorphous intermediate exists and can comprise several competing reactions that can be affected by the reaction conditions and/or the sample history[7, 18-20].
The reactions equations (1.2),(1.3),(1.4) and (1.5) shows the decomposition pathways from temperature 150 °C to 600 °C up to the complete decomposition of γ- Mg(BH4)2. Reaction (1.2) and (1.3) are taken from reference  whereas reactions (1.4) and (1.5) are taken from references [7, 18]
and [7, 19] respectively. From reaction (1.5) it can be seen that completely decomposed γ- Mg(BH4)2
forms MgB2 as the final reaction product and needs gaseous reaction with hydrogen for the reversible reaction as given by [15, 19, 21] and as mentioned in reaction (1.6). According to  it is possible to reabsorb only about 2.5 H2 wt% or only 40% of the desorbed amount. The above reactions (1.2) and (1.3) suggests out of the two phases Mg(BH4)2, only one of these is reversible to Mg(BH4)2, so, this can be one of the reasons for incomplete rehydrogenation. Another reason can probably be the formation of a boron-containing intermediate compound in this partial decomposition process is too stable and prevent the complete re-hydrogenation. However, the formation of MgO at the expense of Mg(BH4)2
might have also been responsible for the reduced reVersibility.
MgB2 +4H2 𝑦𝑖𝑒𝑙𝑑𝑠
→ Mg(BH4)2 (1.6)
But as mentioned in , at 200°C γ- Mg(BH4)2 undergoes reversible re-hydrogenation to triborane Mg(B3H8)2 according to equation (1.7) and yields 2.5 wt% of H2.
↔ Mg(B3H8)2 +2MgH2 +2H2 (1.7) Continuous ball milling of magnesium diborane at 400 °C in a hydrogen atmosphere of 950 bar H2 after 108 hours resulted in 75% of Mg(BH4)2. This product was characterized by TGA-DSC, XRD, IR, and solid- state NMR. Again, the same reaction was carried out at room temperature with 100 bar of H2 pressure for 100 hours resulted in 50% of Mg(BH4)2.
In summary, the partially decomposed γ- Mg(BH4)2 needs lower temperature and pressure to re- hydrogenate than the completely decomposed one but the hydrogen production during re- hydrogenation is only about 2.5 H2 wt% which is not sufficient for the hydrogen storage for fuel cells.
Its reversible hydrogen storage capacity must start from almost 6 H2 wt% provided the moderate reaction conditions. Thus, only knowing that the partially decomposed magnesium borohydride can lead to a reversible reaction with less amount of hydrogen production is not sufficient at the moment
rather it has become very important to understand and find out the intermediate amorphous species in order to improve the hydrogen storage property of Mg(BH4)2. Identifying the intermediate species of the reaction will lead the researcher to the different pathways for the improvement of hydrogen storage. For example, by adding additives like transition metal additives to avoid forming the B-H bond during hydrogenation and dehydrogenation of Mg(BH4)2 or preparing reactive hydride composites with Mg(BH4)2 and/or nanoconfinement .
Figure 1.2: Structure of -Mg(BH4)2, -Mg(BH4)2, and -Mg(BH4)2 (models obtained using the VESTA program). Magnesium atoms are represented with tetrahedra where each vertex is occupied by a
[BH4]- unit and, in all the structures, every vertex is shared between two tetrahedra .
So, the main purpose of this work is to study the reaction products of different reaction steps in Mg(BH4)2 decomposition including the intermediate amorphous products formed in the 240–300°C temperature range. For this purpose, several samples were prepared in the lab in different temperatures and the argon flow of 200 ml/min which were then studied by using X-ray absorption spectroscopy (XAS), and laboratory powder X-ray diffraction (PXD) to characterize the unknown intermediate species.
XAS can find out the composition of these intermediate species by finding out the coordination and the oxidation state of the X-ray absorbing atom in the sample. In the present work, XAS was used to determine the local environment around the boron by obtaining XANES spectra at boron K-edge and this technique was chosen to characterize the partially decomposed amorphous sample because this technique is especially used to probe the amorphous species. Laboratory powder X-ray diffraction (PXD) was used to identify the presence of crystalline species in the samples and characterize them.
As mentioned earlier, the main compounds of interest are amorphous therefore the PXD was mainly used to determine the composition of starting materials. This method has been traditionally applied for phase identification, quantitative analysis, and the determination of structure imperfections .
Samples were prepared using the TGA-DSC instrument. As γ-Mg(BH4)2 is a highly air-sensitive sample it was heated up to the desired temperature in the argon (Ar) environment with the Ar flow rate of 200 ml/min. The TGA device measured the change in weight of the substance as the temperature changed and the weight loss curve subsequently gave the information about the change in sample composition, thermal stability, and the kinetic parameters for chemical reactions in the sample. The DSC measurements and the peaks in the heat flow curve gave information about whether the heat is flowing into or out the sample (i.e. endothermic/exothermic reactions). So, the simultaneous TGA-DSC measures both gave the information on heat flow and weight changes in a material as a function of temperature or time in a controlled atmosphere and helped to simplify interpretation of the result.
The complementary information obtained from TGA-DSC thus allowed differentiation between endothermic and exothermic events which have no association with weight loss directly but could be because of melting or crystallization and those which involve a weight loss (e.g., degradation) .
2.1. X-rays wave-particle duality
X-rays with energies ranging from about 100 eV to 10 MeV (wavelength =10 to 0.01nm) are classified as electromagnetic waves. X-rays are different from the radio waves, light, and gamma rays in wavelength and energy and show wave nature with wavelength ranging from about 10 to 10-3 nm. X- rays can be treated both as electromagnetic waves and as particles. According to quantum theory, the electromagnetic wave can be treated as particles called photons or light quanta .
Figure 2.1: The EM spectrum, showing major categories as a function of photon energy in eV and wavelength .
Since the X-rays can be treated as electromagnetic waves, they can be explained by classical electromagnetic theory (Maxwell equations). So, as an electromagnetic wave, they show interference (X-ray diffraction), reflection, refraction, and polarization phenomena. As electromagnetic wave X-rays travel through space in a sinusoidal fashion and follows the general relation of a traveling wave as stated below.
Decreasing wavelength (λ) = increasing frequency (ƒ) = increasing energy (E)
X-rays also show particle behavior and their particle behavior can well be explained is by Quantum theory (Schrodinger wave equation). As a particle, they can be produced, show the photoelectric effects and the absorption. The phenomenon is called Compton scattering, which proved that X-rays are particles. Hence, Compton scattering can only be understood by taking X-rays as a particle. 
2.2. Production of X-rays
2.2.1. Production of X-rays in Cathode tube:
When a high voltage of several tens of kV is applied between the two electrodes, the high-speed electrons with sufficient kinetic energy are drawn out from the cathode and collie with the anode (metallic target). The electrons rapidly slow down losing their kinetic energy but this kinetic energy losing method for each electron is different, the continuous X-rays with varying wavelengths are generated. When the electron loses all its energy in a single collision, an X-ray with maximum energy is produced with the shortest wavelength. The value of the wavelength limit can be estimated from the accelerating voltage between two electrodes. When the electrons impact the target (the anode), X-rays are produced in two main ways, which is given by:
a) Bremsstrahlung: This form of radiation, ‘ braking radiation’ in German, is explained by the fact that the accelerated electrons, as they hit the anode, are slowed down if they have high energy and the amount of braking (energy) is converted into different forms of radiation. This radiation is diverse and of different wavelengths because, each electron hitting the anode, slows down, and loses its kinetic energy with a different method.
b) Characteristic radiation: This form of energy is produced by the ejection of electrons from either K, L, M etc. orbitals through impacts with other electrons sent from the cathode. Hence a characteristic X-ray emission occurs for specific electron orbits when the energy of incoming electron overcomes the binding energy of the orbital electrons in the target atom [25, 26].
Figure 2.2: The mechanisms of Bremsstrahlung and Characteristic radiation .
15 2.2.2. Production of X-rays in a synchrotron:
Synchrotron radiation is electromagnetic radiation that is emitted when charged particles move at a speed close to the speed of light. In synchrotrons, the moving charged particles are forced to change their direction by using magnetic fields provided by powerful magnets. In nature, synchrotron light can be produced by astronomical objects like crab nebula, which is a supernova remnant in the Taurus constellation. Since the late 1940s synchrotron light has been artificially generated using particle accelerators. Synchrotron radiation covers a wide range of frequency from infrared to the highest-energy X-rays and is characterized by the properties such as high brightness (many orders of magnitude brighter than conventional sources), highly polarization, tunability, collimated beam (almost parallel rays) and concentrated over a small area . This property as a single word can be called brilliance.
Another important property is the energy of the electrons within the storage ring which generates the X-rays, which influences the range of photon energies that any one facility can practically cover . The main advantage of synchrotron light source over the cathode tube is that only the single wavelength X-ray is possible to produce once because the anode target material needs to be chosen and keep fixed in the cathode tube, and this is why it is not tunable resource and also the intensity of the source is less than that of synchrotron 
A synchrotron consists of five main components:
1. The electron gun is a source of electron where the electrons are generated by thermionic emission from the hot filament. These electrons are then accelerated using a linear accelerator (linac) at about 100 MeV. A regular supply of electron is required as they are usually being lost in the machine due to collision with residual gas particles in the storage ring.
2. The electrons from the linear accelerator are then injected into the booster ring where they are further accelerated. Then the electrons are periodically injected to the main storage ring so that the specified storage ring current is maintained.
3. The storage ring contains the array of magnets which makes the electrons move in a closed circular path. These are mainly of three types; dipole or bending magnets which cause the electrons to change their path and thereby follow a closed path. Quadrupole magnets are used to focus the electron beam and compensate for Coulomb repulsion between the electrons and sextupole magnets correct for chromatic aberrations that arise from the focusing by quadrupoles. The electrons have K.E measured in GeV and their velocities are highly relativistic (very marginally less than the velocity of light).
The storage ring contains bending magnets (BMs) and the straight sections used for insertion devices (IDs) which generate the most intense synchrotron radiation.
4. Radiofrequency (RF) supply: To supply the electrons just the right amount of extra energy every time they pass through it to replenish the energy loss by the electrons while emission of synchrotron radiation.
5. Beamlines: The beamlines run tangentially to the storage ring, along the axes of the insertion devices and tangentially at bending magnets. Beamlines have three sections; front end, optics hutch, and experimental hutch. The front end monitors the position of the photon beam, filters out the low-energy tail of the synchrotron radiation spectrum if necessary, etc. The photon beam is then normally focused and/or monochromated in the optics hutch. The hutches are shielded using the lead-lined, thick concrete wall to protect users from not only X-rays but also from gamma rays and high-energy neutrons, which can be produced in the storage ring when the relativistic electrons collide with stray gas particles. Such gamma rays penetrate very deeply in the matter, hence effective radiation shields may consist of tens of centimeters of
lead blocks. Experiments in the experimental hutches are therefore performed remotely, from outside the radiation area .
Fig 2.3: Schematic diagram of the most important components of modern synchrotron source .
2.3. X-ray spectroscopy and Interaction of X-rays with matter:
X-ray spectroscopy is the study of X-ray electromagnetic radiation and its interaction with matter. It is one of the widely used analytical techniques to study the structure of atoms and molecules. The technique is also employed to obtain information about atoms and molecules as a result of their distinctive spectra . We know that the electromagnetic waves carry energy in terms of waves, so when this energy (E= hν) carrying waves like X-rays, strikes the particle, they produce some change in the particle. This interaction is studied by a technique called Spectroscopy. Spectroscopy can be carried out in two ways either by absorption or by the emission of electromagnetic waves. When an electromagnetic wave reacts with matter one can obtain either absorption spectrum or emission spectrum, but the spectrum obtained is determined primarily by the atomic or molecular composition of the material. That is why the spectroscopy technique is extensively used to study the internal structure of the material.
From the application point of view, there are mainly following X-ray spectroscopic techniques.
1. X-ray absorption spectroscopy 2. X-ray fluorescent spectroscopy 3. X-ray emission spectroscopy
Several other techniques can be categorized within three of these techniques .
Figure 2.4: (Right) The interaction of X-rays with matter. (Left) The cross-section for various processes involving the interaction of X-rays with the matter for Barium (Ba) .
Figure 2.4, (right) shows the possible interaction of X-rays with matter. When the X-rays incident on the matter, the phenomena like refraction, reflection, absorption, scattering (elastic scattering = Thomson scattering and inelastic scattering = Compton scattering), diffraction and fluorescence all are possible processes that can take place. If none of the above takes place, the photon is then transmitted through the sample. But for the applications using synchrotron radiation only photoelectric absorption, elastic and inelastic scattering (which also includes diffraction) are important as shown in Figure 2.3. (left). Figure 2.4, (left) shows the cross-section for five different processes that can take place when X-rays interact with matter. The cross-section is given in the unit of barn which is equal to 10-24 cm2. The yellow-colored region indicates the upper energy range covered by synchrotron sources up to some MeV. In this range, two processes dominate, namely photoelectric absorption and elastic (Thomson) scattering, although inelastic (Compton) scattering also becomes significant above 30 KeV. Further in this work, X-ray absorption spectroscopy will be discussed as it is the main focus of this work.
2.4. X-ray Absorption Spectroscopy 2.4.1. Introduction
X-ray absorption spectroscopy (XAS) is a photoelectric effect and one of the spectroscopic tools that are widely used in many research labs to study the geometric and electronic structure of the matter.
It is useful for probing the internal structure of material nanoparticles. Its use has been increased because of the availability of synchrotron radiation facilities around the world.
When X-ray is scanned through matter, it can ionize the target atom by ejecting electrons from any of the core shells such as K or L or M … and so on (which depends on the binding energy of each core shells), then there is the sudden increase in absorption cross-section which appear as peaks in the graph and are called absorption edges.
In XAS, the measurements are made by tuning the X-ray energy at and above a selected core-level binding energy of a specific element. The spectra obtained through this process information about the oxidation state and the coordination chemistry of the selected element. In addition, the extended oscillations of the XAS spectra are sensitive to the distances, coordination number, and species of the atoms immediately surrounding the selected element. When the measurements are carried near and at the binding energy (also called the absorption edge) it is called the X-ray absorption near- edge structure (XANES) and measurement above the absorption edge is called extended X-ray fine Structure (EXAFS).
Each atom and ion has a unique internal structure in terms of the number of electrons, binding energies, and atomic environment. This produces a characteristic X-ray absorption spectrum thus allowing for obtaining valuable information on the atomic geometry, electron density, oxidation state, electronic configuration symmetry, coordination number, and interatomic distances of atoms/ions in different molecules and/or compounds [30, 31]. Absorption of X-rays by an atom can be regarded as causing a fluctuation of the electron energy up to a virtual level. When the X-ray hits the target atom, and if the incoming X-rays have energy greater than the binding energy of core electrons, the probability of ejection of core electrons increases and hence the interaction strength or ‘cross-section’
between X-rays and core electrons increases. This interaction between the X-rays and the core electrons are stronger than those between X-rays and valence electrons. Then there is a role of X-ray absorption spectroscopy (XAS) techniques, which are concerned with the change in response of a system as a function of incident photon energy. XAS experiments can mostly be performed at synchrotrons even though the instruments have appeared recently. So, generally in XAS, a core electron is excited to an unfilled valence state and this state can then relax via emission of a photon or maybe radiation less leading to the ejection of photoelectrons, auger electrons or cascade of low energy secondary electrons [25, 32].
Figure 2.5: The absorption of an X-ray photon proceeds via the ejection of a core electron. This can then be filled by an electron from a shell further out. The excess energy can either be emitted in the form of characteristic X-ray radiation or by the ejection of an Auger electron (left). The three electron
process in Auger emission (right) .
2.4.2. X-ray Absorption process
The photoelectric absorption of X-rays is highly dependent on the atomic number Z (approximately to the fourth power) of an atom absorbing the X-rays. The penetrating power of X-ray is dependent on the energy carried by it and also the Z of that atom . The absorbing power of a material is
determined by its absorption coefficient (µ) which describes the exponential drop in intensity of an incident beam passing through a medium. This absorption coefficient of material depends on the type of atoms in the sample, how those atoms are distributed, the nature of their bonding, light polarization, and the wavelength of X-rays. Let us consider the sample of thickness “d” in the transmission experiment. If “I0” denotes the initial intensity of X-ray beam and “I” denotes the intensity after transmission through the sample of thickness “d”, then the following relation holds,
𝐼𝑜= e-µd (2.1)
Where “µ”, is called the linear absorption coefficient, and the above relation is called the “Beer- Lambert” law of liner absorption . The following equation shows the relation of “µ” with the absorption cross-section per atom (also called total photon interaction cross-section) denoted by
µ = (𝜌𝑚𝑀𝑁𝐴) σa
where NA, M, and ρm are Avogadro’s number, molar mass, and the mass density of an atom.
Figure 2.6: A plot of absorption cross-section vs energy of incident photon for different elements [33, 34]
2.4.3. Quantum Mechanical treatment
The scattering event in quantum mechanics is defined by the time-dependent perturbation theory.
The interaction between the incoming beam and the sample is then defined by the Hamiltonian of interaction, Hf, as the transition from an initial state|i⟩ to a final state ⟨f|. It is also given in first-order perturbation theory by Fermi’s Golden rule, the number of transitions per-second W:
W = 2π
ℏ |Mif|2ρ(εf) (2.3)
With the matrix elementMif =⟨i|Hf|f⟩andρ(εf)being the density of states. The absorption process is not elastic, meaning that the incident photons expels an electron from an atom with binding energy
𝜀𝑝𝑒 = ℏ2𝑝2
𝜀𝑝𝑒 is the kinetic energy of the photo-electron and is equivalent to the difference between
εbe the energy of the incident photon. In this case, there are no restrictions over the direction of the wave vector of the photoelectron
, 𝑞⃗and thus, is enough to perform the integration over the entire solid angle of∆Ω=4π.
ℏ |𝑀𝑖𝑓|2𝜌(𝜀𝑝𝑒)𝛿 (𝜀𝑝𝑒− (𝜀 − 𝜀𝑏)) 𝑑𝜀𝑝𝑒
(2.5) The density of states for the photoelectron is eValuated in the same way as for scattering events, using the so-called box normalization .
𝜌(𝜀𝑝𝑒) = 2 ( 𝑉
8𝜋3) ( 𝑑𝒒 𝑑𝜀𝑝𝑒)
(2.6) Here factor 2 allows for the two possible spin states of the electron, while the volume element 𝑑𝒒 is replaced by 𝑞2sin(𝜃)𝑑𝑞𝑑𝜃𝑑ɸ. It is now possible to define the absorption cross-section as:
4𝜋3∫|𝑀𝑖𝑓|2𝛿 (𝜀𝑝𝑒− (𝜀 − 𝜀𝑏)) 𝑞2sin(𝜃)𝑑𝒒𝑑𝜃𝑑ɸ
(2.7) with ɸ0= 𝑐/𝑉 the incident flux. It also now defines the factor 𝑀𝑖𝑓(calculation details can be retrieVed in book  as:
𝑀𝑖𝑓 = ⟨𝑓|𝑒 𝑚 𝒑. 𝑨|𝑖⟩
(2.8) Here the terms 𝒑 𝑎𝑛𝑑 𝑨 are introduced, which indicate the momentum operator and the vector potential, coming from the interaction Hamiltonian
.The expression is then obtained by neglecting the Coulomb interaction between the photo-electron on the positively charged ion left behind. (i.e. free-electron approximation)  .
188.8.131.52. Free-electron approximation:
It is now brieﬂy reported the derivation of the free-electron approximation for the calculation of the absorption cross-section (full treatment can be read in ). The initial state |𝑖⟩is deﬁned as one photon described by the couple (k,𝜀̂) being respectively its wave-vector and its polarization, and one K electron: |i⟩ = |1⟩x |0⟩e. The ﬁnal state |𝑓⟩is represented instead by the annihilated photon and the photo-electron expelled by the absorption process: |𝑓⟩ = |0⟩x |1⟩e. It is then found the state for which the electron is free as eigenfunction of p with eigenvalueℏ𝐪:
21 𝑀𝑖𝑓 =𝑒ħ
2𝜖0𝑉𝜔 (𝒒. 𝜀̂) ∫ Ψ𝑒,𝑓∗ 𝑒𝑖𝒌.𝑟Ψ𝑒,𝑖𝑑𝑟
(2.9) where r is the position vector of the photo-electron and Ψ its wave-function. The square root term is the normalization factor A0, which turns out from the quantization of the vector potential A. It is now considered for the approximation that the initial wave-function of the electron is taken to be that of the 1s bound state, while the ﬁnal wave-function is of a free electron. These conditions are written respectively as:
𝛹𝑒,𝑖 = 𝛹1𝑠 (r)
𝛹𝑒,𝑓 = 1
It is also deﬁned the wave-vector transfer by 𝑸 = 𝒌 − 𝒒, and it's integral as ɸ(Q), the Fourier transform of the wave-function of the electron in its initial state. This makes it possible to eValuate the squared matrix element,
2𝜖0𝑉2𝜔(𝑞2 𝑠𝑖𝑛2𝜃 𝑐𝑜𝑠2ϕ)ɸ2(𝑸) (2.11)
and thus the absorption cross-section per K electron by substitution of the matrix element in the equation:
where I3 is a three-dimensional integral, about which deﬁnition and evaluation is skipped for convenience (however it can be found in the literature ), however, it is found to be reduced to the quantity (4
the following quantities are deﬁned as:
• ℏωK: The energy of the absorption edge, proportional to Z2 for a simple model
• ℏωA: The energy related to K, the inverse length scale of the wave-function Ψ1s, proportional to Z
• ℏωc: The highest characteristic energy, deﬁned as ℏωc =2mc2
and hence the ﬁnal result for the atomic absorption cross-section per atom:
;for ℏωK << ℏω << ℏωc
This makes apparent that the absorption cross-section varies as Z5 via ωA, and as ω−7/2 via the factor of 𝜆 = 2𝜋𝑐/𝜔. This result is slightly diﬀerent from the experimental ﬁndings, summarized in Fig. 2.6.
The reason for this diﬀerence is caused by the approximation made for the free-electron, implying the Coulomb interaction between the photo-electron and the positively charged ion to be neglected.
However, in this way, it was available to obtain an analytical approximate expression for 𝜎𝑎  .
184.108.40.206. Beyond the free-electron approximation:
In this part, we will further show a step in the calculation of the absorption cross-section.
The dimensionless photon energy variable is given by:
ξ = √ω−ωωk
and it is conveniently possible to write his result as a correction factor f(ξ) for the absorption cross- section per K electron:
σ𝑎= 32𝜆𝑟0(43) [ ω ω ω𝐴2
(2.15) This correction factor is dependent on both Z and ℏω, and its explicit form can be written as:
𝑓(ξ) = 2 𝜋√ω𝑘
1−𝑒−2 𝜋ξ )
(2.16) it is useful at this point to consider two interesting limits;
1. When the photon energy is greater than the binding energy: ℏωK >> ℏω or ξ→ 0, it follows that f(ξ) →1.
This returns the same result for the free- electron approximation: If the photon energy is high, so the energy of the photo-electron and it makes a little difference if it is free to move, or it is in a weak attractive field produced by the positive ion.
2. When the photon energy is approaching to threshold energy: ℏω -> ℏω+, ξ→ ∞, it follows that f(ξ) → 2𝜋𝑒4
At the threshold energy, there is thus a discontinuous jump of : σ𝑎= 32𝜆𝑟0(4
3) [ ω𝐴2
ω ω 𝑐]
5 2(2 𝜋
To calculate the values for ωA and ωK, needed for the ealuation of the energy dependence and the step height in 𝜎𝑎 at the K-edge, it uses the approach of the hydrogen atom. In this way, the K shell ionization of an atom with Z electrons is approximately the binding energy of the hydrogen atom times Z2: ℏ ωK = 𝜋𝑎𝑍2𝑒2
0𝜖02 while ℏ ωA =𝑍ℏc𝑎
It is, therefore, possible to write the edge jump per K electrons as:
σ𝑎(𝜆𝑘) ≃ (256𝜋
3𝑒4) 𝜆𝑘𝑟0 (2.18)
and energy dependence as:
σ𝑎≃ 32𝜆𝑟0(43) [ω ω 𝑘]
4(2 𝜋𝑒4) (2.19)
the results that are shown in the last two (write the name of the equations) are proven to be reliable, as compared to recent experiments and more detailed and refined frameworks.
2.4.4. Absorption edges
When the X-rays are scanned through the target material, one can see the abrupt increase in the absorption cross-sections in the particular energy ranges of an incident photon. This happens when the energy of a scanned X-ray corresponds to the binding energy of the core-shell electrons and the corresponding peaks are said as K-edge, L-edge, M-edge, and so on, with each edge representing the different core- electron binding energy. The table below shows the absorption edges and the orbital electrons responsible for it.
Table2.1: Absorption edges and corresponding electronic transitions
Figure 2.7 shows three major transitions in Pb (K, L, and M edges), corresponding to the excitation of an electron from n= 1, 2, and 3 shells, respectively. At higher resolution, both the L and M edges are split . When there occurs the resonance of X-ray photon energy with the ionization threshold of K or 1s state, this results in K-edge and does not have any sub edges (which L or M can have). The reason for not seeing sub edges in K-edge is that the orbital angular momentum (l) for K orbit is zero and therefore there can be no coupling, which is possible in L or M edges where the orbital angular momentum is not zero .
Figure 2.7: (a)Low-resolution X-ray absorption spectrum for Pb . (b) Atomic orbital labeling .
Thus, X-ray absorption spectroscopy (XAS) is the measurement of the X-ray absorption cross-section in the vicinity of one or more absorbing edges. X-ray absorption edge is a very- important part of the X-ray absorption spectrum because it is not only the discontinuous increase in absorption, but it shows the significant structure both in the immediate vicinity of the edge jump (XANES) and well above the edge (EXAFS) which can extend up to more than 1,000 eV. The absorption edge region, which is within
Absorption edges Electron Transition states
L- edge 2s 2p
M- edge 3s 3p 3d
N- edge 4s 4p 4d 4f
the 50 eV of the main edge, is divided into three sub-regions namely, the pre-edge region, the main edge region, and the post-edge region. Before the main edge, sometimes it is possible to observe some small peaks which are called pre-edge structures. The main region where the abrupt increase in the cross-section is observed is called the absorption edge and the immediate region after the main edge which extends up to few eV, having very little fluctuation in absorption cross-section is the post-edge region. The Post-edge region is the region before the EXAFS region.
X-ray absorption near-edge structure (XANES) is a type of absorption spectroscopy that indicates the features in the XAS spectra of compounds due to photoabsorption cross-section for the electronic transition from the atomic core level to final states, in the vicinity of the absorption edge of an atom.
Most importantly, the ability to make qualitative fingerprint-like comparisons of XANES spectra is making it a very useful tool to find out the information about the unknown substance. If a representative library of reference spectra is available, spectral matching can be used to identify an unknown. Beyond this qualitative application, there are three main ways in which XANES spectra are used: to determine the oxidation state, to deduce three-dimensional structure, and as a probe of electronic structure  around the X-ray absorbing atom. This technique uses synchrotron radiation to provide the spectra containing valuable information. In XANES, a photon is absorbed, and an electron is excited from a core state to an empty state. To excite an electron in a given core-level, the photon energy has to be equal or higher than the binding energy of this core-leVel. This gives rise to the opening of a new absorption channel when the photon energy is scanned. The energy of an absorption edge, therefore, corresponds to the core-level energy, which is the characteristic for each element, making XANES an element-selective technique.
In XANES, X-ray ejects the core electron to the empty shell of an atom and generates the core hole and the process is dominated by Fermi- Golden rule which gives the probability of transitioning from initial states to the final states of the ejected photoelectron. When the dipole approximation is taken into account, it applies the selection rules as,
where l is the orbital angular momentum quantum number and the selection rule states that only the following transition is available giving rise to the specific edges.
1s → K-edge 2s, 2p → L-edges 3s, 3p, 3d → M-edges 4s, 4p, 4d, 4f → N-edges
One can also have quadrupole transition (l = ±2) but they are very week and are not significant  . The absorption edge is more complex than just an abrupt increase in absorption. There are weak transitions below the absorption edge in the pre-edge region. The pre-edge is strongly affected by the bond lengths of the molecules because of exponentially decay of wavefunctions, and the edge is to indicate the ionization energy of the core hole.
Physically during experiments, when the energy of X-ray matches or exceeds the binding energy of core electrons, those electrons get ejected or occupy unfilled valence shell and the vacant space of
these electrons are recovered either by photoemission or by the emission of auger electrons and hence electric current generated from these auger electrons are measured as a function of incident energy.
Figure 2.8: XAS spectrum showing important regions of XANES, namely pre-edge, main-edge, post- edge, and the EXAFS region 
The pre-edge region in XANES spectra is because of the electronic transitions to the empty bound stage (transitions probability controlled by dipolar selection rules). For example, 1s→ 3d or 1s→ 4p is the transitions in 1st transition series metals. This region contains information about the local
coordination environment around the absorbing atom, but this information is dependent on the oxidation state and the bonding of the compound in the study. The main edge peak defines the ionization threshold to continuum states and gives the information about the main edge shifts to higher energy with increasing oxidation state.
2.4.6. Interpretation of XANES
1. The sensitivity of XANES to Oxidation state
Edge spectra even though frequently have unresolved transitions superimposed on the rising edge, have proven extremely useful in determining the oxidation state of the absorber. This may be explained by using an electrostatic model since atoms with a higher oxidation state should have a higher charge, thus requires an energetic X-ray to eject the electron from its core. An alternative interpretation treats the edge features as ‘’continuum resonance’’. A continuum resonance involves the excitation of a core electron into the state above the continuum that has a finite lifetime. This phenomenon correlates the edge energy and oxidation state of the compound of interest and hence is widely used in coordination chemistry.